TESTS OF PRESTRESSED CONCRETE BEAM SPLICES
JOINT HIGHWAY RESEARCH PROJECT PURDUE UNIVERSITY AND INDIANA STATE HIGHWAY COMMISSION
Final Report TESTS OF PRESTRESSED CONCRETE BEAM SPLICES
Gutzwiller, Research Engineer and
R„ H, Lee, Research Engineer
Joint Highway Research Project File Nos
This research investigation was conducted in cooperation and with the assistance of the Indiana State Highway Commission and the Prestressed Concrete Producers of Indiana
Purdue University Lafayette, Indiana July 25, 1969
Digitized by the Internet Archive in
2011 with funding from
LYRASIS members and Sloan Foundation;
Indiana Department of Transportation
Final Report TESTS OF PRESTRESSED CONCRETE BEAM SPLICES
J. F. McLaughlin, Director Joint Highway Research Project
July 25, 1969 File No: 7-4-16
H. L. Michael, Associate Director
Project No: C-36-56P
Joint Highway Research Project
The attached Final Report entitled "Tests of Prestressed Concrete Beam Splices" has been prepared by Professors M„ J, Gutzwiller and R. Ho Lee of our staff. The study was performed with the assistance and cooperation of the Indiana State Highway Commission and the Prestressed Concrete Producers of Indiana, The report contains the lesults of tests made on three types of prestressed beam splices. An analysis and discussion of the tests for each type is presented. The Prestressed Concrete Producers of Indiana wish to obtain of these reports and release of the report to them is requested.
Harold L. Michael Associate Director
Ashbaucher W. L. Dolch w. H. Goetz w. L. Greece F. L.
G. K. Ha Hock M. E. Harr
R. Ho J. A. V. E. F. B. R. D.
Harrell Havers Harvey Mendenhall Miles
Scholer Scott M. B. Spencer W. I C.
H. R. J. Walsh K. B. Woods E. J. Yoder
Bridge span lengths have been steadily increasing throughout history, caused by changing technology and design criteria
A typical example of
changing criteria may be found in the Interstate Highway construction program, which presently accounts for
large volume of bridge work.
Safety standards now used in bridge design require bridge abutments to be
located considerably farther from the pavement edge than previously.
This change in criteria
coupled with standard median widths, roadway widths
etc, requires span lengths of around 100 feet for overpasses having no skew.
As span length requirements increase, changes in technology are
needed to economically fulfill the new criteria.
Prestressed concrete beams have been used in of the bridge superstructures.
In the United States, most of the pre-
stressed concrete work has been accomplished with precast beams, manufactured at
fixed plant and transported to the construction site for
The beams are commonly pretensioned
i.e., the prestressing
tendons are stretched between permanent anchorages.
Concrete is then
placed in the forms and cured, bonding to the steel.
The tendons are
then released, compressing the concrete.
Pretensioning requires massive
extensive handling facilities and concrete batching machinery.
A large capital outlay is inherent, and the operation is well suited for mass production methods. The sequence of events is slightly different in the manufacture of
post-tensioned beams. a
Concrete for post-tensioned members is placed with
void space for the tendons.
After the concrete has gained sufficient
strength, the tendons are stressed by jacking against the beam itself.
In general the terms pre and post refer to the timing of the tendon stress-
ing operation, either before or after concrete placement.
does not require
large fixed plant, but the method is not readily
amenable to mass production of beams.
It may be used efficiently for
casting of large members. Since most prestressed concrete work in the United States is accom-
plished by pre -tensioning, the problem of transportation to the construction site remains.
Bridge spans of 100 feet or more require transportation
of rather long members, usually over the public highways.
passages of long members might be considered as occasional events, highway
authorities are becoming more reluctant to grant over- length permits on daily, continuing basis.
Hauling restrictions for prestressed beams indicate
the need for field splicing of the precast members when long spans are
encountered. The Prestressed Concrete Institute recognized the need for splicing and presented
number of possible field splices in a recent publication.
However, the available test data on how certain of these splices function are somewhat limited.
The Prestressed Concrete Producers of Indiana
which is an organization of manufacturers, would like to use some of these splices in future bridge work.
producer's association undertook splice types.
In order to determine splice behavior, the a
full scale test of three different
The actual design of the splices was done in the Bridge
Design Section of the Indiana State Highway Commission.
Beams were fabri-
cated by Construction Products Corporation in Lafayette, Indiana.
were performed at the company's casting yard.
The tests were monitored by
staff members of the Joint Highway Research Project at Purdue University.
(1) "Prestressed Concrete
Concrete Institute, 1968.
for Long Span Bridges" published by Prestressed
One specimen of each splice type was tested,, on May 15, 1969, with
The three tests were made
number of manufacturer representatives, state
highway and other interested personnel present. Each splice type is described separately in the report. details, test procedure, results and discussion are given.
Construction It should
be pointed out that the beam lengths chosen were dictated by the testing
frame and equipment.
The beams are essentially full size for the span
lengths on which they were tested.
40 foot test
span to a 120 foot field span should not incur any unexpected results.
Design calculations for the various splices are not included in this report.
If information on these calculations is desired, contact the Bridge
Design Section, Indiana State Highway Department, Indianapolis
POST- TENS IONED SPLICE
One type of splicing situation which may arise is indicated in Figure 1.
The use illustrated is that of a simple span beam, spliced in the region (There are other possible configurations where this
of high bending moment.
splice may prove useful.) The splice connects two precast beams by using post- tensioning cables
threaded through ducts in the adjoining members.
A thin layer of grout
between the two beams is used to provide an even bearing surface. are temporarily shored while the cables are threaded, a
cast-in-place deck slab placed.
removal of the shores. beams.
the grout packed
The cables are then stressed, permitting
Grouting of the void space bonds the cables to the
The post-tensioning cables provide the connecting link between the
The precast beams contain a miner amount of pre-tensioning
steel to prevent cracking during handling and transportation.
HYDRAULIC JACK REACTING AGAINST LOAD FRAME
GROUT LAYER BETWEEN PRECAST BEAMS 2
SPLICE - LOAD
Details of Test Beam The test beam had an overall length of 51 '-0".
was used, with end blocks to facilitate transfer of the concentrated post-
tensioning forces at the ends.
placed in the end blocks.
Extra stirrups and a reinforcing grid were
beam details in section and elevation.
show the load arrangement and
Two post-tensioning cables were
used, each containing 9-%" diameter strands
were 278 kips per cable. span.
270 kip grade.
The cables were draped parabolicaliy through the
Four 7/16" 270 kip pre-tensioning strands were provided for handling
The beams were made on May 7, 1969.
The grout layer was two inches wide and was placed on May 9, 1969.
5'-0" wide slab, 7" thick, was cast to simulate the deck that would be used in the prototype.
Stirrups extending through the top of the beam provided
shear connection to the slab.
Concrete was mixed in the batch plant of Construction Products
gives the cylinder strengths obtained for the concrete
in the beams and composite slab.
Concrete Cylinder Strengths Post- tensioned Splice
6" x 12" Cylinder compressive strengths
*Average of three cylinders At the time of testing, beams were old.
days old and the slab was
The grout layer between beams was placed
days prior to testing.
post-tensioning cables were stressed and grouted 24 hours prior to the test. While no cylinder strengths were obtained for the grout, it appeared that the
19 9 2.2
STRAND -PULLED TO KIPS
CAST- IN- PLACE
EACH POST-TENSIONiNG CABLE! 9- /Z $ STRANDS (273* JACK.iNG FORCE) [
2-6 END BLOCK
POST-TENSIONED SPLICE -DETAILS
grout was not of good quality.
It was rather soft and could be removed by
When the cables were stressed,
appeared in the concrete slab directly over the grout joint, extending from the top of the slab to a depth of about 6 inches.
0.06" at the top.
Crack width was about
Theoretical stress calculations at this point indicated
compression throughout the depth of the member.
Apparently the grout had
much lower stiffness modulus than the slab concrete, causing the grout to shorten more under compression than anticipated. material at the splice was not of
In other words, the grout
stiffness comparable to the other com-
ponents, as assumed in the original stress analysis.
Initial upward camber after post-tensioning was 2.44 inches at the
centerline of span.
Test P rocedure The specimen was loaded through a hydraulic jack at the centerline of the span.
The jack reacted against a steel test frame boLted to the foundation.
Elastomeric bearing pads were used at the end bearings and between the jack and the slab.
The jack had a capacity of 400 kips, while the test frame was
rated at about 200 kips.
The jack had been pre-calibrated for correspondence
between gage pressure and applied load. Load values which are given in the results are values taken from the jack calibration charts.
A separate load transducer was not used, due tc
the demonstrative nature of the tests.
Load values given are probably within
-5 percent and depend primarily on the accuracy of reading jack gage pressure.
At the beginning of the test, the gasoline engine for the hydraulic
pump was started. crease.
A valve was used to control the hydraulic pressure in-
Loads were applied in 10 kip increments to 30 kips.
working load range for the member.
was then released, new zero readings taken, and the load was reapplied in
load of 70 kips had been reached, the load
was again released to zero.
A third loading stage then was carried to
Information obtained during the test consisted of vertical deflections,
number and spacing of cracks, crack width, and the overall failure pattern.
Vertical deflections were measured at the centerline and quarterpoints of the span using
Short pieces of level rod were
attached to the beam at the deflection points. each load level with an accuracy of 0.005
Readings were taken at
feet or about 1/16 inch.
tions at the quarter points were essentially symmetrical and an average
value of these readings is used on the accompanying plots.
Figure 4 gives
the load-deflection response of the beam. The
member exhibited two basically linear load deflection ranges
below 30 kips and
second region of reduced stiffness above about 40 kips.
Cracking of the beam under load was confined to an extremely localized region at the splice.
single crack at one edge of the grout
interface was the only visible crack until just prior to failure, when two
few inches on either side of the splice.
Cracking first appeared at
load of 20 kips and was of hairline width.
At 30 kips the crack had progressed to approximately the mid-depth of the web As the applied load increased and the crack width became significant, the
width was measured with
hand rule to the nearest 1/16 inch.
shows the load-crack width relation observed in the test.
Preliminary calculations by the Bridge Design Section indicated ure load of 110 kips with a completely bonded cable.
unbonded cable was calculated at 59 kips, using
Failure load for an
formula for steel stress at
I09 K MAX.
100— QUARTER - POINT
POST-TENSIONED SPLICE- LOAD VS. DEFLECTION
POST-TENSIONED SPLICE- LOAD
failure from the American Association of State Highway Officials (AASHO)
design specifications a
This formula is extremely conservative and represents
lower load limit on observed failures with unbonded tendons.
Actual failure of the beam came at
load of 109 kips.
The beam would
not accept greater load and deflected until the jack reached maximum extension.
During this time the crack widened on the tension side and gradual progressive
crushing of the concrete occurred on the top fibers.
Deflection of about
0.6 foot at the centerline was obtained and crack width was about
shows an elevation view of the splice region of the beam
failure, while Figure
is a close up view
of the splice itself.
of the grout layer separated completely from the beam and dropped out.
Discus sion of Results
Results of this splice test were somewhst clouded by the relatively poor grout strengths which were obtained. ing beams apparently did not cure to
The grout layer between adjoin-
strength or stiffness comparable to
the beam and slab concrete, as evidenced by the slab cracking which occurred.
It is certain that this deficiency could be easily corrected with proper
A more serious drawback to the post-tensioned splice was the lack cf adequate bond between the cables and the beam.
Casting two beams separately
and joining them in a region of maximum bending moment automatically creates a
weakened plane where cracks may be expected.
With insufficient bond
between the cable and beam, the cable elongations tend to be concentrated at the splice point
large crack width, as evidenced in this test.
It might be argued that improved tendon grouting (and therefore improved
bond) would automatically alleviate the crack width problem by distributing the cracks along the member and reducing the average width.
test can neither confirm nor disprove that supposition.
The results cf the
POST-TENSIONED SPLICE AT FAILURE
CLOSEUP VIEW OF POST-TENSIONED
present test indicate that excessive crack width at working loads can occur
with the splice as constructed. Another factor to be considered in evaluating tests of this type is that the test involved only
few load cycles
Progressive loss of bond
due to repeated loading in a highway bridge could also cause excessive crack
widths The ultimate load capacity of the member compared very closely to the
predicted value (109 kips vs. 110 kips).
The prediction was made using the
AASHO equation for bonded steel stress at failure.
It should not be implied
from this close agreement that the cables were bonded at failure.
of Figures 6 and failure.
shows the magnitude of slip which had to occur prior to
A more reasonable interpretation of the failure load data is that
the beam properties were such that large steel elongations were present at
The average steel strain at failure was therefore high and the fail-
ure load approached the bonded value.
Based on the test described above, it appears that the post tensioned splice should not be used in regions of high bending moment where excessive
crack width at working loads is
Further tests might establish that proper cable grouting would solve the crack width problem by creating better crack distribution.
Construction of continuous spans by splicing several units often done by placing the splice near in Figure 8.
point of inflection, as illustrated
The concept may be easily extended to multiple spans.
splice would normally be used in regions of relatively small bending moment,
but would be subjected to fairly high shears.
CAST-IN-PLACE SPLICE— GENERAL
The splice contemplated in the present application consists of
place concrete section of perhaps 4 feet in length, reinforced with mild steel bars projecting from each precast element.
also used in the splice.
Supplemental stirrups are
(Possible variations would include post-tensioning
the cast-in-place portion, but this will not be considered herein.)
If this type of splice is placed near a dead-load point of inflection,
one design condition of importance would be the possibility of live load
causing splice moments of differing sense.
If certain positions of live
load cause tension on the top and other positions cause tension on the bottom, the need for splice steel en both faces should be considered.
described herein was reinforced on one side only.
Construction of the splice in the field would entail supporting the precast units on temporary shores, forming and pouring the splice, and finally casting the deck slab.
Details of Test Beam The test specimen had an overall length of 43 -0". F
and span length are shown in Figure 9.
near the quarter-point of the span. the precast beam.
The cast-in-place splice was placed
Figures 10 and 11 show the details of
Figure 12 shows the details of the cast-in-place joint.
The member was tested as a simple beam having
concentrated load at the center of the span.
caused high shear at the splice, along with
span length of 40*-9", The loading arrangement
relatively high bending moment
while this condition would rarely occur in field usage, it is certainly more stringent test of the splice.
large amount of mild steel was
placed in the splice to carry the anticipated bending moment.
gages were placed on the mild steel bars at locations shown in Figure 13.
29-10" Igjj STIRR. -DRAPE 6
MIDPOINT />;]. lie • •
STRANDS TO 2000
©@. ©A •
- 270 k STRAND
PULLED 22 - 46
2 3 '2
Construction of the test beam was made by forming the precast elements in a prestressing bed and using a blockout in the splice region.
bars (embedded 2'-0" into the precast beam) projected through the blockout area.
The precast elements were pre-tensioned with straight and deflected
cables which ran continuously through the blockout.
After curing of the pre-
cast elements, the pretensioning cables were cut off at each end of the precast elements.
The remainder of the splice reinforcement was then placed.
Beams were cast on April 24 and the splice was placed on April 29.
concrete was placed on April 30. Table
The member was tested on May 15.
gives the cylinder compressive strengths obtained for the
concrete used in the various pours.
Concrete Cylinder Strengths
6" x 12" Cylinder compressive
Cast-in-Place Splice strength
* Average of three cylinders
An epoxy bonding compound was specified on the ends of the precast elements to
facilitate bond between the beam and splice concrete..
ning of the test,
Prior to the begin-
hairline crack was observed at each end of the joint
concrete over the entire depth of the member.
These were apparently shrink-
Test Procedure The specimen was loaded x^ith the hydraulic jack and loading frame
described previously. and at the load point.
Elastomeric pads were provided at the end bearings
Loading was applied in 20 kip increments, up to 60 kips, after which 10 kip increments were used.
An unloading cycle was not used.
Provisions were made to measure the strains at several points on the mild steel in the splice.
Vertical deflections were measured, and the crack-
ing pattern and failure behavior were observed.
Sixteen metal film strain gages were attached tc the mild steel splice bars in pairs at the points indicated in Figure 13. are also designated in the figure. for steel
A dummy gage on
Gage reference numbers
The gages were temperature compensated
steel bar embedded in
concrete cylinder was
used; three-wire leads to each gage minimized temperature effects due to the lead wire lengths. a
Gages were waterproofed with an epoxy compound and
technique which disturbed only
small portion of the bond surface of
Gage number 16 was not operative at the start of the test and gage
Strains in the remaining gages were
number 11 was damaged during the test.
measured at various load levels using operated strain indicator.
Budd Type p-350 portable battery-
Reading accuracy was -5 micro-inches per inch.
The strain data obtained are given in Table
load versus steel strain for the various gages.
Figure 14 is
Each gage strain plotted is
the average of two gages at the same location, one each on the top and bottom
of the bar.
are averaged, as are 3 and 4, etc.
r 9 a 10